A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks


 Horace Glenn
 1 years ago
 Views:
Transcription
1 Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints and permissions: sagepub.co.uk/journalspermissions.nav DOI: 0.77/ jcm.sagepub.com Chandra Veer Singh and Ramesh Talreja, Abstract We treat selected test cases in the third world wide failure exercise by the approach described as synergistic damage mechanics. This approach utilizes micromechanics and continuum damage mechanics to predict the overall mechanical response of composite laminates with ply cracking in multiple orientations. The material constants needed in the continuum damage mechanic formulation are calculated from stiffness property changes incurred in a reference laminate. For other laminate configurations, the stiffness changes are derived using a relative constraint parameter which is calculated from the constraint on the opening displacement of ply cracks within the given cracked laminate evaluated numerically by a finite element analysis of appropriately constructed representative unit cell. The number density of ply cracks (cracks per unit length normal to the crack planes) under quasistatic loading is calculated by an energybased approach. Finally, the stress strain response of a laminate is determined by combining stiffness property changes and evolution of crack number density. Keywords Synergistic, continuum damage mechanics, cracks, unit cell Introduction and historical background Failure analysis of composite materials is currently performed by the industry using empirical criteria, none of which properly accounts for the effects of damage processes prior to complete failure. Significant developments in the past three decades suggest that accounting for subcritical damage will improve composite design. While previous exercises, focused on the ultimate failure, the third world wide failure exercise (WWFEIII) provides an opportunity to examine initiation and progression of subcritical events and their effect on the mechanical response. In composite laminates, which are the subject of examination in WWFEIII, the damage initiation processes begin at the constituent level within a ply. In most cases, ply cracks span the thickness and width of the ply at relatively low loads. Subsequent loading then results in multiplication of these cracks. It is common, therefore, to start the analysis with assumed presence of ply cracks and examine their evolution (increase in number per unit length normal to crack planes) as well as the effect of these cracks in changing the laminateaveraged mechanical properties. The approaches taken to address this problem can be broadly characterized as microdamage mechanics (or simply, micromechanics), e.g. shearlag methods, see for example References [4 ], and continuum damage mechanics (CDMs). Our current approach is to retain the framework of CDM but enrich its capabilities by combining it with micromechanics. We have called this approach synergistic damage mechanics (SDM). The present paper will first briefly describe the SDM methodology and then apply it to selected cases of WWFEIII. The CDM 7,8 uses a physically based damage characterization that does not leave behind essential features of damage in the context of the material response of Department of Materials Science and Engineering, University of Toronto, Toronto, ON, Canada Department of Aerospace Engineering, Texas A&M University, College Station, TX, USA Visiting Professor, Luleå University of Technology, Luleå, Sweden Corresponding author: Ramesh Talreja, Department of Aerospace Engineering, Texas A&M University, College Station, TX , USA. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
2 Journal of Composite Materials 0(0) interest while keeping in sight practical implementation of the resulting methodology. As argued in References [7,8] and elaborated further in References [9 ], a scalarvalued characterization would be inadequate in view of the oriented nature of the internal surfaces formed. Although a vectorvalued characterization was employed at first, the issue of ambiguity of the sense of a vector could be addressed more elegantly by using a second order tensor instead. The damage characterization for ply cracking involved calculation of a constraint parameter,, which essentially captures the environment of the cracked surfaces (e.g. effect of surrounding plies), and a number of damage constants, c i which depend on the laminate material. These constants will be described later. The observation that the parameter may be viewed as a carrier of the local effects on damage entities within a Representative Volume Element (RVE), while the c i constants are material constants, led to a number of studies to explore prediction of elastic property changes due to damage in different modes. To be sure, the elastic properties are the averages over appropriate RVEs. CDM model considered here predicts effective stiffness changes for the whole laminate; layerwise (or laminawise) CDM model have also been developed., At first it was found that from changes in E x and xy due to transverse cracking in [0/90 ] s glass/epoxy laminates reported in Reference [4] and assuming no changes in E y, changes in E x for the same glass/epoxy of [0/90] s configuration could be predicted with good accuracy. Also, in [0/45] s laminate of the same glass/ epoxy, the change in E x could be predicted by setting damage parameters D(þ45) ¼ D(45) (a good approximation, supported by crack density data). These results have been reported in Reference [9]. Later, a systematic study of the effect of constraint on the constraint parameter was done by experimentally measuring the crack opening displacement (COD) in [/90 ] s laminates 5 7 for different  values. By relating these values to the COD at ¼ 90 and normalized by a unit applied strain, the predictions of E x and xy for different could be made. Another study of the constraint effects was made by examining [0/ 4 / 0/ ] s laminates, where the ply orientation was varied. Once again, using experimentally measured COD for ¼ 90 as the reference, the parameter for other ply orientations was evaluated from the COD values and E x and xy for different were predicted. 8 While the experimental studies supported the idea of using the constraint parameter as a carrier of local constraints, the scatter in test data and the cost of testing do not make the experimental approach attractive. Therefore, another systematic study of [0 m / n /0 m/ ] s laminates was undertaken 9,0 where computational micromechanics was employed instead of physical testing as a means of evaluating the constraint parameter. An elaborate parametric study of the constraint parameter allowed developing a master curve for elastic property predictions. The most recent study examines damage modes consisting of transverse ply cracks as well as inclined cracks of different orientations in [0 m / n /90 r ] s and [0 m /90 r / n ] s laminates. The SDM approach is developed and its predictions are compared with available experimental data for [0/90/45/þ45] s laminate. At the current state of its development, the SDM methodology has the ingredients of a multiscale damage mechanics depicted in Figure. As illustrated there, structural (macroscale) analysis of a part containing damage is accomplished by a mesoscale SDM analysis of appropriate RVE in which microscale input from micromechanics (computed CODs) as well as materials constants from a reference laminate configuration are entered. What remains is to codify this approach in software to be used by design engineers. Theoretical details Definition of damage Consider a continuum body of a composite solid with a matrix and embedded reinforcements as well as a multitude of damage entities in the form of microcracks. In CDM, the material microstructure, e.g., distributed fibres, and the distributed damage, which may be called the microdamage structure, are treated as smearedout fields. For evaluating the effective properties of the continuum body, the continuum is homogenized using a twostep homogenization procedure (see Figure ). As illustrated in the figure, the material microstructure is viewed as consisting of stationary entities, e.g., fibres and plies, and the microdamage structure is considered as a family of evolving entities, e.g., cracks and voids. First the stationary microstructure is smeared into a homogeneous, anisotropic material. In the next step, the evolving microstructure is replaced by a homogeneous field represented by suitable internal variables. The internal microdamage structure evolves with loading and causes changes of the overall response (properties) of the composite. Resorting to Figure again, consider a generic point P inside the damaged composite body. Let an element of volume V contain a representative sample of damage entities about this point. An individual damage entity (a crack or a void) can be viewed as bounded by a surface S, on which any point can be associated with two vectors, one of which, a, represents a selected influence of the damage entity, and the other, n, is the unit outward normal to the surface. Let the surface integral of dyadic product of the vector components a i n j be Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
3 Singh and Talreja Figure. Multiscale synergistic methodology for analyzing damage behaviour in a general symmetric laminate [0 m / n /90 r ] s with matrix cracks in þ, and 90 layers. Stationary microstructure RVE for damage characterization Evolving microstructure Step Homogenization of stationary microstructure P Step V Homogenization of evolving microstructure P a i n j Continuum after homogenizing the stationary microstructures Fully homogenized continuum Characterization of a damage entity Figure. Homogenization of a continuum body with damage. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
4 4 Journal of Composite Materials 0(0) denoted by the secondorder tensor components d ij. Thus, Z d ij ¼ a i n j ds s The total set of damage entities may be divided in subsets of entities having same geometrical characteristics (orientation, shape, etc.) and termed as damage modes. For example, matrix cracks may constitute one damage mode, while fibre/matrix debonds may constitute another. Also, matrix cracks in different orientations may be grouped into different damage modes. Assuming that there are N damage entities of a given mode a in the RVE, the damage mode tensor is defined by D ðþ ij ¼ X V k d ij k where k ¼,,..., N and V is the volume of the RVE. Let us now focus on the particular case of intralaminar cracking in composite laminates. Figure shows an RVE illustrating one set of intralaminar cracks in an offaxis ply of a composite laminate. Although for clarity of illustration, the cracking is shown only in one lamina, it is understood that in general it exists in multiple plies of the laminate. The thickness of the cracked plies is denoted by t c, s is the average crack spacing, t is the total laminate thickness and W and L stand for the width and the length, respectively, of the RVE. The volume of the RVE, the surface area of a crack, S, and the influence vector magnitude, a, are specified as V ¼ L W t S ¼ W t c sin a ¼ t c where, called the constraint parameter, is an unspecified constant of (assumed) proportionality between a and the crack size t c (also crackedply thickness). Here, 0 p/, so that S is always positive. Assuming a to be constant over the crack surface S, one gets from equation () ðþ ðþ ðþ The synergistic damage mechanics methodology For the mechanical response of a damaged body in isothermal condition, the Helmholtz free energy function is given by 9 ¼ " ij, D ðþ Helmholtz free energy is thus a function of the damage state. The energy change brought about by damage is represented by terms involving D ðþ ij. The stress tensor is then given by ij ij ij where m is the mass density. For a linear elastic homogenized body, ij ¼ C ijkl " kl where the stiffness matrix C ijkl is given in the Voigt notation as C pq ¼ C 0 pq þ X C ðþ pq where C 0 pq is the initial (undamaged) stiffness matrix and P C ðþ pq represents the stiffness changes brought about by all the damage modes. In the following, we consider the different cases of cracking in composite laminates and derive the corresponding damagestiffness relations. Case : Only 90 ply is cracked (single damage mode). Let us consider the Helmholtz free energy for a composite laminate with its 90 ply cracked. As shown before, 8 0 a polynomial form is most suited for our formulation. Assuming the composite laminates in consideration to be orthotropic, the form of the polynomial must remain invariant with respect to the coordinate transformations expressing this symmetry. Such restrictions to polynomial functions are satisfied by making use of certain polynomial invariants called the irreducible integrity basis.,4 Considering a single damage mode, ¼, we have the following set of invariants ", ", ", ", ", ", " " " ð5þ ðþ ð7þ ð8þ D ðþ ij ¼ t c st sin n in j where n i ¼ ðsin, cos, 0Þ. ð4þ D, D, D, D, D, D, D D D " D, " D, " D, " " D, " " D, " " D, " D D, " D D, " D D ð9þ Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
5 Singh and Talreja 5 Figure. A representative volume element illustrating intralaminar multiple cracking in a general offaxis ply of a composite laminate. This set of integrity bases can be further reduced for the case of a thin laminate loaded in its plane. For such laminates, only the inplane transformed strain and damage tensor components need be considered. Thus, the remaining integrity bases in the Voigt notation for thin laminates are given by where ", ", " D, D, D " D ð0þ " "," "," ",D D,D D,D D : The most general polynomial form for Helmholtz free energy, restricted to secondorder terms in the damage strain components and first order terms in damage tensor components (low volume fraction of damage entities), is given by ¼ P 0 þ c " þ c " þ c " þ c 4" " þ c 5 " D þ c " D þ c7 " D þ c 8 " D þ c 9 " D þ c 0 " D þ f c " " D þ c " " D g þ fc " " D þ c 4 " " D gþp ð" p, D q ÞþP ðd q Þ ðþ where P 0 and c i, i ¼,,..., 4 are material constants, P is a linear function of strain and damage tensor components and P is a linear functions of damage tensor components. Setting the free energy to zero for unstrained and undamaged material, we have, P 0 ¼ 0, and assuming the unstrained material of any damaged state to be stressfree, we get P ¼ 0. The stress Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
6 Journal of Composite Materials 0(0) components in the Voigt notation are now given by (from equation ()) p p where p ¼,,. From () and (), we have where p, q ¼,,, and C pq ¼ C 0 pq þcðþ pq c c 4 0 C 0 pq ¼ c Symm c E 0 0 x xy E0 y 0 xy 0 yx 0 xy 0 yx ¼ E 0 y 0 xy 0 yx 4 Symm 0 0 G 0 xy 7 5 ðþ ðþ ð4þ represents the orthotropic stiffness matrix for virgin composite material, where E 0 x, E0 y, 0 xy, G0 xy are effective moduli for the undamaged laminate (calculated using CLT), and c 5 D þ c D pq ¼ 4 c 7 D þ c 8 D c 4 D c D þ c D c D C ðþ 7 5 Symm c 9 D þ c 0 D ð5þ represents the stiffness change brought about by the damage entities for damage mode. For the special case of laminates with cracks in only 90 plies, we obtain ( ¼ 90 ) C ð90þ pq ¼ t c st 4 a a a 0 5 ðþ symm a wherea i, i ¼,..., 4 are material (laminate) constants to be determined from experimental or computational data on stiffness degradation. It can be observed that the orthotropic symmetry is retained by intralaminar cracking in crossply laminates. In the above relations, ð the constraint parameter ¼ u Þ t c where u and tc represent the COD averaged over the crack surfaces and the thickness of the cracked 90 layer, respectively. The engineering moduli for the cracked laminate can be obtained from the following relationships: E x ¼ C C C C E y ¼ C C C C xy ¼ C C G xy ¼ C Thus, for laminates with 90 ply cracks only, E 0 x E x ¼ 0 þ Da xy 0 yx E 0 y E y ¼ 0 þ Da xy 0 yx xy ¼ 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 y 0 þ Da xy 0 yx G xy ¼ G 0 xy þ Da where " # 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 y 0 þ Da xy 0 yx " # D ¼ t c st 0 xy E0 y 0 þ Da 4 xy 0 yx E 0 x 0 þ Da xy 0 yx ð7þ ð8þ ð9þ As seen from equation (8), the shear modulus is uncoupled from the other three moduli and thus can be treated independently. The four constants appearing in these relations are evaluated by using initial elastic properties and their values at one crack spacing. Thus, if the chosen crack spacing is s 0, then " # a ¼ E x E 0 x D 0 xy yx 0 xy 0 yx " # E 0 y a ¼ E y D 0 xy yx 0 xy 0 yx a ¼ h i G xy G D 0 xy 0 " # a 4 ¼ xy E y 0 xy E0 y D 0 xy yx 0 xy 0 yx with D 0 ¼ D s¼s0 ¼ t c s 0 t. ð0þ Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
7 Singh and Talreja 7 Case : multiple damage modes. The details of damage modeling in multidirectional laminates with cracking in multiple offaxis plies are given in References [9 ] and reproduced in Appendix A for the sake of completeness. For the special case of [0 m / 90 r / n ] s and [0 m / n /90 r ] s laminates with intralaminar cracks in þ, and 90 layers, the stiffnessdamage relations are same as in equation (8) except that D is now given by 8 D ¼ t 0 t s n ð þ rþ 904nþr r 90 þ r 90 n j ¼90 s 90 ðþ with the following constraint parameters ¼ u 4n ; 904nþr ¼ u 90 4nþr ; 90 ¼ u 90 r 4nt 0 ð4n þ rþt 0 rt 0 ðþ for [0 m /90 r / n ] s laminates, and D ¼ 4t 0 t s n ð þ rþ 904nþr r 90 þ r 90 n j ¼90 s 90 ðþ with the following constraint parameters ¼ u n ; 904nþr ¼ u 90 4nþr ; 90 ¼ u 90 r nt 0 ð4n þ rþt 0 rt 0 ð4þ for [0 m / n /90 r ] s laminates, where t 0 is the thickness of a single ply, s n, and s90 are the normal crack spacings in and 90 plies, respectively. In expressions for the constraint parameters, the subscript denotes a particular damage mode (orientation of cracked plies) and subsubscript represents the number of cracked plies corresponding to that damage mode. The flow chart in Figure describes the procedure for multiscale synergistic methodology for multimode damage assessment taking an example of [0 m / n /90 r ] s laminates. Computational micromechanics involves analysis of a representative unit cell to determine the COD values and the constraint parameters. In a separate step, the material constants a i appearing in equations (8) and (0) are determined from experiments or numerical simulations carried for a reference laminate, specifically [0/90 ] s. These relations are then employed to predict stiffness degradation with constraint parameters and material constants obtained from experiments (or FE simulations) as inputs. In the final step, the overall structural behavior in response to external loading can be analyzed based on the degraded stiffness properties for the damaged laminate. A reference laminate in principle could be any crossply laminate of a chosen configuration. The procedure for predicting crackinginduced property changes for other crossply laminates is independent of this choice. The specific choice of [0/90 ] s laminate was made here as experimental data for this laminate was available from which the constrained parameter could be estimated. The procedure described above for determining elastic moduli changes in a laminate requires calculating CODs of ply cracks. However, the laminate elastic moduli can change additionally due to the nonlinear shear response of plies. In References [8,0] a procedure for correcting the CDM predictions by including this response was illustrated. Modeling of damage evolution For predicting evolution of ply cracking, the authors have developed an energybased approach, which is capable of dealing with cracking in offaxis plies of orthotropic laminates. In Reference [5], the approach is described and applied to several ply cracking cases. Here, we apply it to the relevant WWFEIII test cases. A brief description of the approach follows. As illustrated in Figure 4, two damage states are considered: State with N parallel offaxis cracks spaced at distance s, and State where the cracks have multiplied to N and attained spacing s/. The crack density is assumed to increase when the work required in going from State to State (which is the Figure 4. Progressive multiplication of intralaminar cracks in an offaxis ply. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
8 8 Journal of Composite Materials 0(0) same as work needed to close N cracks in going from State to State ) exceeds a critical value, i.e., if in a general offaxis ply, one can use a multimode criterion given as W N!N N:G c sin t c ð5þ M þ w N II ðþ w I G Ic G IIc where is the offaxis angle shown in Figure and G c is the critical (threshold) value of energy required for ply crack formation within the given laminate (more discussion about this later). The work required to form additional N cracks in going from State to State is therefore, W N!N ¼ W N!0 W N!0 ðþ where W N!0 and W N!0 represent work required to close N cracks in State, and N cracks in State, respectively, and the two quantities are calculated as (see Reference [] for detailed derivation) W N!0 ¼ N sin ðt cþ h ð0 E Þ : ~u n ðsþþ i 0 ~u n ðsþ W N!0 ¼ N sin ðt cþ : E ð7þ h ð0 Þ: s ~u n þ 0 ~u s i t ð8þ where ~u n, ~u t are the normalized average crack opening and sliding displacements (COD and CSD). These are given by ~u n ¼ u n t c 0 =E ¼ t c 0 =E ~u t ¼ u t t c 0 =E ¼ t c 0 =E Z t = t c = Z t = t c = u n ðþdz z u t ðþdz z ð9þ where u n and u t represent the relative opening and sliding displacement of the cracked surfaces, respectively, and overbars represent averages. For the special case of cracking in 90 ply only, the sliding displacement is zero (under uniaxial loading condition) and hence the criterion for ply multiplication is written as 0 h t c : ~u s i n ~u n ðsþ G Ic E ð0þ where G Ic is the critical energy release rate in Mode I (crack opening mode). This is the same relation as derived for cracking in crossply laminates by Joffe et al. except that they consider centrally placed cracked 90 plies in their model and normalize the average COD with half the ply thickness (t c /). For cracking where w I ¼ ð 0 Þ E w II ¼ ð 0 Þ t c E h : ~u s i n ~u n ðsþ ; h : ~u s i t ~u t ðsþ ðþ and G IIc is the critical energy release rate in Mode II (crack sliding mode), and the exponents M and N depend on the material system, for example, for glass/ epoxy M ¼, N ¼. 5 In our work, 5 we interpret the critical material parameters G IC and G IIC not in the usual linear elastic fracture mechanics sense where they are defined as the resistance to advancement of the crack front at the point of unstable crack growth. Instead, we postulate that the work required to go from State to State involves a range of dissipative processes that all depend on the material condition in a cracking ply within the given laminate. The material parameter representing the dissipated energy per unit of ply crack surface is, therefore, not what is obtained in a standard fracture toughness test for determining G Ic or G IIc. Furthermore, as discussed in Reference [5], we believe a ply crack cannot form unless sufficient energy is available to open its surfaces (i.e. mode I). In other words, a pure sliding action will not generate a set of parallel cracks illustrated in Figure 4. This will imply that the second term in equation () is negligible. In fact, we report good predictions of crack density evolution by only using the first term in equation (). Also, we do not use the conventional G Ic but extract this value from test data of a reference laminate and use it to make predictions for other laminates. For the WWFEIII, however, we are given conventional G Ic and G IIc and have used those. Thus, the predictions reported here will not be in accordance with our analysis proposed in Reference [5]. Analysis method The prediction of overall stress strain response for a given damaged laminate using CDM entails following steps:. Determine damage constants a i that appear in the damagestiffness relations (equation (8), using equation (0)). This task requires stiffness constants Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
9 Singh and Talreja 9 for virgin (undamaged) laminate, E 0 x, E0 y, G0 xy, v0 xy, and moduli of cracked laminates at some specified crack spacing, s 0 : E x ðs 0 Þ, E y ðs 0 Þ, G xy ðs 0 Þ, v xy ðs 0 Þ. The moduli for virgin laminate are obtained through the classical laminated plate theory (CLT) by using the properties of a unidirectional lamina, whereas their values at crack spacing s 0 are obtained by micromechanical analysis using finite element method (FEM) for reference laminate [0/90 ] s. In earlier works, e.g., References [8,0], these constants were obtained using experimental data for stiffness changes. It is noted here that the choice of a reference laminate is driven by convenience and availability of experimental data. Since in earlier works 8,0 the [0/90 ] s laminate was used to obtain the material constants, the same laminate was then used in later work as the reference laminate for FEM calculations.. Find stiffness constants as a function of crack density ( c ¼ /s) using equation (8), depending on the laminate type. This gives, C ijkl ¼ f ð c Þ ðþ. Predict evolution of crack density as a function of applied axial strain using the fracture criterion expressed in equation (0). Thus, c ¼ f " ij ð4þ The strain to initiation of first multiple cracking can be estimated by backward extrapolation of the function f. 4. Combine results from steps and (equations () (4)) to obtain stiffness properties as a function of applied strain, equation (5), and predict the overall stress strain response of the laminate for axial tensile loading along laminate longitudinal direction. C ijkl ¼ c ijkl " ij ð5þ Computational micromechanics (FE analysis). As described above, SDM approach requires evaluation of COD and damage constants, experimentally or computationally. Since the BVP for multidirectional laminates is inherently threedimensional, we use D FE analysis to compute these parameters. For the reference crossply laminate, the representative unit cell is as shown in Figure 5. For this laminate layup, periodic boundary conditions are applied to the end faces in the transverse (y) direction, and laminate symmetry about the midplane is achieved by having outofplane displacements (w) zero at the symmetry plane. Uniform displacement is prescribed on the right face of the cell to have tensile loading. However, for multidirectional laminates with cracks in more than two orientations (e.g. multimode cracking in [0/90/þ/] laminates), the construction of FE model is somewhat complex and is detailed in References [,5]. For SDM predictions for laminates, we chose [0/90 ] s, i.e. ¼ 90, as a reference laminate. The stiffness damage results for this crossply laminate can be obtained in a variety of ways. The most obvious way would be by using experimental data. However, although experiments reflect the real material behaviour, they can be performed for limited cases. An alternative and more general way is to use a numerical tool such as an FE model to simulate stiffness degradation. FE simulations are in fact easier to carry out and have no scatter other than the accuracy of computations that may depend on mesh density and implementation of boundary conditions. The crack density along x direction (or equivalently, the crack spacing) was varied by changing the length of the unit cell considered. Linear elastic FE analyses were carried using ANSYS 7 for the reference laminate. The cracks were assumed to be fully grown through thickness and width of 90 plies. The longitudinal modulus and the Poisson s ratio of the damaged laminate were obtained using the volume averaging 8 of stresses and strains as given by Figure 5. Representative unit cell for FE analysis of reference [0/90 ] s laminate. The applied displacement boundary conditions are shown above. Periodic boundary conditions are applied on end faces in the width (y) direction. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
10 0 Journal of Composite Materials 0(0) the following equations h E x ¼ xxi h i " xx xy ¼ " yy h i " xx ðþ ð7þ where brackets <> specify volume averaging. CODs averaged over thickness of the cracked ply are calculated from u ¼ t c Z tc= t c = u ðþdz z ð8þ where u ¼ u þ u represents the separation of crack planes in the direction normal to the crack face in the local lamina coordinate system x, x, x with x along crack longitude, x transverse to the crack and x along ply thickness. Numerically, u is determined from nodal x direction displacements averaged over the entire crack surface. The above micromechanical expressions are exact in the sense that they do not involve any homogenization theory and are directly calculated from FE data. Errors in the calculations can be only due to approximation in FE analysis. Further details on FE analysis methodology and validation for multidirectional laminates can be found in References [0,,5,9,0]. It should be pointed out here that we have not included thermal stresses caused by cooling down of the composite laminates to the room temperature. However, it can be easily taken into account during prediction of damage evolution by including thermal stresses, which are calculated here by classical laminate plate theory (CLT). We demonstrate the effect of thermal stresses on one of the test cases: Test case 4. The coefficient of thermal expansion is assumed to be constant during entire loading process. Hence, we neglect any change in thermal expansion brought about by ply cracking. Theoretical prediction of the WWFEIII test cases The SDM model, by itself, is limited to the prediction of effect of subcritical damage (matrix cracking, for the present scenario) on the stiffness properties of the laminated structure. Unlike the lamina failure theories, it cannot predict the lamina or laminate failure. Hence, our analysis here is limited to the test cases where effect of damage on the stress strain response is desired. The test cases, thus analyzed are Test Case, Test Case 4, Test Case, Test Case 7, Test Case 8, Test Case and Test Case. The input data for the analysis performed here is taken from Reference []. In the first step, we carried out FE simulations to characterize stiffness properties for reference laminate [0/90 ] s for all material types. Thickness of a single ply is taken as 0.5 mm. The crack density for these calculations in simulations was taken to be equal to.0 cr/ mm. Axial tensile loading along laminate longitude was applied to the representative unit cell shown in Figure 5. The changes are thus assumed to occur only in E x, and v xy, where as E y and G xy are assumed to be impervious to damage for this laminate layup. The relative stiffness properties, constraint parameters, D 0, and the corresponding damage constants for three material systems, viz. Glass/epoxy (Glass/LY55), G4 800/ 50 and IM7/855 targeted in this study, are shown in Table. These constants were assumed to be the same for different test cases as long as the ply material remains the same. To evaluate the stiffness changes for various test layups, the constraint parameters were obtained in each case for crack density equal to 0. cr/mm (see Tables and for calculated COD values for different test cases). Then using expressions in equation (8), stiffness properties for other laminates were obtained. In doing so, it must be emphasized that since the damage constants are laminatedependent, they must be adjusted in case the thickness of the cracked ply in the laminate configuration changes, e.g., for Test Table. Stiffness properties and constraint parameters for reference [0/90 ] s laminates made for different materials. The relative stiffness changes are determined from FE simulations at crack density equal to cr/mm, whereas the constraint parameters are calculated at an assumed initial crack density equal of 0. cr/mm Material type Constraint parameter, D 0 E x =E 0 x v xy =vxy 0 Damage constants, a i (GPa) a a a a 4 Glass/epoxy (Glass/LY55) 7.e 4.8e G4800/50 5.5e.8e IM7/ e.5e Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
11 Singh and Talreja Case 4: [0/90 4 ] s laminate, a 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; a ½0=90 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; Š s ½0=90 Š s C 0 C 0 a 0 ¼ a ðc 0 Þ ½0=90 4 Š s ; a ½0= ¼ a ðc 0 Þ ½0=90 4 Š 4 s ð9þ Š s ½0=90 Š s C 0 C 0 where ai 0 represents reevaluated constants for the laminate in consideration and a i represents constants for the reference laminate. Thus, the constants a i s are recalculated every time the relative thickness of layers in the laminate changes. To simulate the stress strain response, we need damage evolution predictions. For this purpose, an Table. Calculated average COD values for 90 cracking for selected test cases. All COD values are in mm Crack density (/mm) Test Case Test Case 4 Test Case Test Case 7 Test Case COD: crack opening displacement. Table. Calculated average COD values for 90 cracking for Test Cases and. All COD values are in mm Crack density (/mm) Test Case Test Case, m ¼ Test Case, m ¼ Test Case, m ¼ COD: crack opening displacement. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
12 Journal of Composite Materials 0(0) Figure. Stiffness and Poisson s ratio degradation for Test Case : [0/90/0] T glass/epoxy laminate. Figure 7. Stress strain response and crack density evolution for Test Case : [0/90/0] T glass/epoxy laminate. No thermal effects were taken into account. energybased fracture criterion given in equation (0) was utilized in a MATLAB code. The normalized average COD and CSD for different crack spacing were obtained using FE simulations on the representative unit cell for the respective laminate. For 90 cracking, the calculated COD values are tabulated in Table (CSD ¼ 0 for 90 cracks). Polynomial fits to these COD values were used in the simulation for damage evolution. The damage evolution subroutine was run until the applied strain reaches longitudinal failure strain in tension. If the calculated crack initiation strain comes out to be higher than the longitudinal failure strain, the laminate is understood to have failed by fibre fractures. Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
13 Singh and Talreja Figure 8. Stiffness and Poisson s ratio degradation for Test Case 4 [0/90 8 /0] T glass/epoxy laminate. For stiffness changes, the damage model considered in the present study is a linear model with respect to the crack density. A nonlinear model will involve additional damage constants and would be required to achieve a better accuracy for high crack density. For present purpose of illustration, a linear approach is sufficient. Test Case. For this test case, Figure shows the variation of longitudinal Young s modulus and the Poisson s ratio normalized with initial values E x, xy E 0 x 0 xy against the normalized crack density ( 90 t 90 ). The evolution of crack density and corresponding stress strain response are shown in Figure 7. For this laminate case, the ply cracks initiate in 90 plies at an applied axial strain of about.%. After initiation, cracks grow in number very quickly on increase in applied strain and reach a saturation level subsequently. The overall shape of crack density increase is parabolic. The value of 90 t 90 reached at longitudinal tensile failure strain (" T ¼ :807%) for this material is slightly more than.0, suggesting a very high value of absolute crack density (8 cracks/mm). Still the effect on stress strain response is not too severe as would be for thicker 90 plies (such as in the next Test Case). Although the Poisson s ratio reduces, its effect on the transverse stress strain curve ( x vs. " y ) is almost negligible. Test Case 4. For this test case, the laminate material is same as in the previous one. However, the thickness of the 90 plies is eight times of that in the previous case. Consequently, the degradation in the laminate stiffness due to ply cracking is much more severe in the present case (see Figure 8). Also, the ply cracks in 90 plies initiate at much lower applied strain of about 0.7%. As compared to the Test Case, however, the rate of damage evolution is lower in this case and the value of 90 t 90 reached at " x ¼ " T for this material is 0., suggesting much lower absolute crack density (0. cracks/ mm). The shape of the damage evolution curve is quite similar to that in Test Case (Figure 9). The stress strain response (also in Figure 9) is significantly nonlinear after ply cracking. For thicker cracked plies, thus, ply cracking may cause severe nonlinearity in the longitudinal stress strain response. Although there is large reduction in the Poisson s ratio subsequent to ply cracking, its effect on the transverse stress strain curve ( x vs:" y ) is not visible. Here, we also illustrate the effect of thermal residual stresses on ply cracking and the resultant stress strain response. Due to differential thermal expansion of longitudinal and transverse plies, the inner 90 ply will develop compressive thermal residual strains when it is cooled from curing to the room temperature. The residual thermal strains due to thermal effects during curing are calculated using CLT as " th t 0 E ¼ t 0 E þ t 90 E T 45: ¼ :4 8: 4 : þ 45: ð Þ0 ð0 5Þ ¼ : :07% ð40þ where t 0 is 0 ply thickness, and T ¼ T ref T service with T service ¼ 5 C being the service (room) Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
14 4 Journal of Composite Materials 0(0) Figure 9. Stress strain response and crack density evolution for Test Case 4: [0/90 8 /0] T glass/epoxy laminate. Dashed lines (denoted in legend by second subscript t) include the effect of strains generated due to thermal mismatch between 0 and 90 plies during curing on damage initiation and progression. temperature, T ref ¼ 0 C being the curing (stress free) temperature. The crack initiation strain thus decreases by 0.07% from the earlier value obtained without considering thermal effects. The rate of damage progression is however independent of thermal residual stresses. Thus, the new damage evolution curve just gets shifted to the left of the curve without such effects by an amount equal to thermal residual strain. The stress strain response is also affected as shown in Figure 9 by dashed lines (using second subscript t in legend). Thermal effects are observed to be small for transverse stress strain response. Test Case. For multidirectional laminates, the damage will form in multiple plies of different orientations. For the specific case of quasiisotropic laminates considered here in Test Cases 8, the cracks may form in 90, þ45 and 45 layers. The combined effect of these cracks is felt more severely on the overall stiffness properties. Although most of stiffness degradation comes from 90 cracks, 45 cracks may interact with 90 cracks and cause more severe degradation than what would be observed if cracks in these different damage modes occurred without affecting each other. SDM model is capable of dealing with this multimode damage scenario, as depicted by stiffnessdamage relationships with D described in equations () (4). Obviously, the density and opening displacements of intralaminar cracks in a given layer will depend on the material, orientation and the thickness of that ply and also on the relative constraint on the cracked ply from surrounding supporting plies. For oblique cracks, sliding of the cracked surfaces will also play a role in the cracking criterion according to equation (). It is often observed in experiments, for example Reference [0], that 45 cracks may not grow fully before the laminate fails by delamination, and therefore we will assume 45 cracks are halfdeveloped, i.e. while evaluating stiffness properties we will reduce the total crack density 45 such that the effective crack density in these plies is given by ð 45 Þ eff ¼ r 45 ; r ¼ 0:5. More detailed information about the growth of cracks is necessary to model this behaviour. This relative density is chosen for illustration purpose only and is based on our experience with model s usage to predict stiffness degradation in quasiisotropic laminates for experimental data on quasiisotropic laminates reported in Reference []. The respective crack densities in different cracked plies are obtained using the damage progression model. Actual experimental observations may be necessary to simulate real material behaviour more accurately. The resulting plots for longitudinal Young s modulus and Poisson s ratio for Test Cases, predicted using expressions in equations (8) and (), are shown in Figure 0. The constraint parameters for 45 cracking with respect to that for 90 cracking are calculated using the parametric equation developed for COD variation with respect to ply orientation in Reference [0] Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
15 Singh and Talreja 5 Figure 0. Variation of longitudinal Young s modulus and Poisson s ratio: (a) vs. normalized crack density in 90 ply and (b) vs. applied strain for Test Case : [0/90/ 45/þ45] s glass/epoxy laminate. Cracks in all offaxis modes are accounted depending on their respective initiation strains and variation of crack densities with applied strain as shown in the next figure. No thermal effects were taken into account. considering cracking in cracking in [0//0 / ] s Glass/epoxy laminates: u ¼ u 90 sin ð4þ Also, it is assumed that 904nþr ¼ 90 and j ¼90 ¼ 90. It is noted that the above equation may not be accurate when cracks in multiple offaxis orientations are present with different crack densities. A more detailed FE computation with experimentally observed crack densities is warranted in such a case. The COD variation in 45 plies is assumed following equation (4). As a simplification, the cracking in both 45 plies is assumed to initiate at identical applied strain and progress with same rate, although experiments may suggest that the 45 ply that is adjacent to 90 ply may fail earlier. In Figure 0, we first show the variation of laminate stiffnesses with respect to crack density in 90 ply. Because at higher applied strains cracks are present in all offaxis orientations, Figure 0(b) is more appropriate, which shows their variation with respect to the applied strain. The damage progression in all offaxis plies is shown in Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
16 Journal of Composite Materials 0(0) Figure. Stress strain response and crack density evolution for Test Case : [0/90/ 45/þ45] s glass/epoxy laminate with cracks in all offaxis modes. The crack initiation and the crack density evolution in both 45 plies are assumed to be identical. No thermal effects were taken into account. Figure. Stiffness and Poisson s ratio degradation for Test Case 7: [0/ 45/þ45/90] s G4 800/500 laminate. Figure. The cracks initiate in 90 ply at about 0.% axial strain, and in 45 plies at about.5% axial strain. Initial stiffness degradation (" x 4 0:%) occurs due to 90 cracks only, whereas later (" x 4 :5%) 45 cracks also contribute to stiffness degradation. The evolution curves for normalized crack densities in 95 and 45 plies have similar shapes, with saturation levels of 90 t 90 0:7; 45 t 45 0:. No thermal effects were considered while predicting damage progression and resultant stiffness properties. As a result of ply cracking in multiple orientations, the stiffness degradation is more severe than would be for cracking in 90 plies only. As reported in Reference [], cracks in 45 plies will typically form from 45/90 interfaces and tend to further enhance opening of cracks present in 90 plies. This increases the rate of Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
17 Singh and Talreja 7 Figure. Stress strain response and crack density evolution for Test Case 7: [0/ 45/þ45/90] s G4 800/500 laminate with cracks in 90 plies only. Strains generated due to thermal mismatch between 45  and 90 plies during curing were taken into account while evaluating damage initiation and progression. damage evolution as well as corresponding degradation in stiffness properties and is not accounted for here. Some nonlinearity is observed in longitudinal and transverse stress strain curves (Figure ). Test Case 7. For this ply material, we observed that our FE calculations on reference laminate [0/90 ] s showed very small relative degradation in E x but significant degradation in v xy (see Table ). The COD, hence the constraint parameter, was also calculated to be smaller with this material. Therefore, the changes in longitudinal Young s modulus are less pronounced for laminate with this material than Glass/epoxy. Figure shows the predicted changes in stiffness properties for this case. The corresponding stress strain response along with crack density evolution is shown in Figure. For laminates made from G4800/50 material, thermal residual stresses generated during curing were found to affect the damage initiation behaviour significantly. For the present layup [0/45/þ45/90] s, the mismatch in axial thermal strains between the 45 and the 90 plies during curing is calculated as 0.%. This decreases the crack initiation strain in 90 plies to about 0.9% (Figure ). The model does not predict any cracking in 45 plies. The shape of crack density evolution is about the same as before with maximum normalized crack density in 90 plies at about 0. at " x ¼ " T. Appreciable nonlinearity is seen in stress strain responses, especially the transverse stress strain response. Test Case 8. When only mechanical strains were considered, our model did not predict any cracking for this laminate (i.e. crack initiation strain for this case was determined to be greater than the provided failure strain for unidirectional lamina). However, when we include residual thermal strains, the cracking in 90  plies is predicted. The reduction in the longitudinal stiffness and Poisson s ratio is predicted to be similar to Test Case 7 (Figure 4) when absolute crack densities are considered. However, the crack initiation and progression behaviour (Figure 5) is quite different mainly due to different thicknesses of 90 plies in the two test cases. For the present case, the mismatch between 0 and 90 plies is important, which is calculated as 0.%. This decreases the crack initiation strain to about.% in 90 plies. Cracks do not form in 45  plies. The normalized crack density is found to rise quickly and the maximum normalized crack density at " x ¼ " T is predicted to be about 0.5, much smaller than that in the Test Case 7. Some nonlinearity in stress strain responses due to cracking is observed. Test Case and. Although these test cases are meant for compressive and tensile strength of the quasiisotropic laminates in the presence of hole, we do not attempt full analysis and prediction here since that would require detailed structural stress analysis. However, we illustrate how SDM model could be applied to laminate cases where ply thickness varies. For given ply layup [45 m /90 m /45 m /0 m ] s in Test Case, we vary m Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
18 8 Journal of Composite Materials 0(0) Figure 4. Stiffness and Poisson s ratio degradation for Test Case 8: [45/0/90/45] s G4 800/500 laminate. Figure 5. Stress strain response and crack density evolution for Test Case 8: [45/0/90/45] s G4 800/500 laminate with cracks in 90 plies only. Strains generated due to thermal mismatch between 0  and 90 plies during curing were taken into account while evaluating damage initiation and progression. from to 4 with m ¼ 4 equivalent to the Test Case. Cracking in only 90 plies is assumed and the analysis neglects any damage in the 45 and 0 plies. If there is significant cracking in 45 plies, the COD calculations (FE model) as well as stiffness predictions must account for cracks in these offaxis plies also, as was illustrated before in case of Test Case 7. Since the ply sequence and relative thickness of cracked and constrained plies remains the same, the relative stiffness change will be given by the ratio of constraint parameters, i.e. ¼ = 0, where 0 is the constraint parameter obtained for the reference laminate [0/90 ] s. is calculated to be 0.555,0.55, and , respectively, for m ¼ to 4. Thus, the stiffness degradation should be the same in all laminates because their relative thickness is the same; the slight difference may be due to different mesh densities and inaccuracies in COD calculations. The ratio of Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
19 Singh and Talreja 9 Figure. Stiffness and Poisson s ratio degradation for Test Case : [45/90/45/0] s IM7/855 laminate. For Test Case, [45 m / 90 m / 45 m /0 m ] s laminate, with different m values, the stiffness reduction is about the same because relative thickness of cracked and constraining plies remains constant. Cracking only in 90 plies is assumed. Figure 7. Stress strain response and crack density evolution for Test Case : [45/90/45/0] s IM7/855 laminate with cracks in 90 plies only. No thermal effects were taken into account. degraded to original longitudinal modulus and Poisson s ratio for m ¼ 4 (Test Case ) is shown in Figure. However, the change in thickness has a significant effect on crack initiation and progression. The crack initiation strain decreases as the cracked ply thickness increases. The rate of damage progression is higher for lower m. For a ply thickness of 0.5 mm (m ¼ ), crack initiation strain was calculated to be.79%, which is greater than the longitudinal tensile failure strain (" T ¼.55%) for the UD lamina with this material. Thus, for this value of m and the provided G Ic value, our model predicts no ply cracking before Downloaded from jcm.sagepub.com at UNIV TORONTO on January 5, 0
A Higher Order Synergistic Damage Model for Prediction of Stiffness Changes due to Ply Cracking in Composite Laminates
Copyright 23 Tech Science Press CMC, vol.34, no.3, pp.227249, 23 A Higher Order Synergistic Damage Model for Prediction of Stiffness Changes due to Ply Cracking in Composite Laminates Chandra Veer Singh,2
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More information1 Durability assessment of composite structures
1 Durability assessment of composite structures 1.1 Introduction Composite structures for mechanical and aerospace applications are designed to retain structural integrity and remain durable for the intended
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationEFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION
EFFECT OF THERMAL FATIGUE ON INTRALAMINAR CRACKING IN LAMINATES LOADED IN TENSION J.Varna and R.Joffe Dept of Applied Physics and Mechanical Engineering Lulea University of Technology, SE 97187, Lulea,
More informationFracture Mechanics, Damage and Fatigue: Composites
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue: Composites Ludovic Noels Computational & Multiscale Mechanics of Materials CM3 http://www.ltascm3.ulg.ac.be/
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationCoupling of plasticity and damage in glass fibre reinforced polymer composites
EPJ Web of Conferences 6, 48 1) DOI: 1.151/epjconf/1648 c Owned by the authors, published by EDP Sciences, 1 Coupling of plasticity and damage in glass fibre reinforced polymer composites R. Kvale Joki
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationMicrocracking, MicrocrackInduced. Delamination, and Longitudinal
NASA Contractor Final Report Microcracking, MicrocrackInduced Delamination, and Longitudinal Splitting of Advanced Composite Structures John A. Nairn University of Utah Salt Lake City, Utah Prepared for
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationHygrothermal stresses in laminates
Hygrothermal stresses in laminates Changing environment conditions (temperature and moisture) have an important effect on the properties which are matrix dominated. Change in temperaturet and moisture
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationMODELING DYNAMIC FRACTURE AND DAMAGE IN A FIBERREINFORCED COMPOSITE LAMINA WITH PERIDYNAMICS
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Mechanical & Materials Engineering Faculty Publications Mechanical & Materials Engineering, Department of 011 MODELING DYNAMIC
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationDamage initiation and evolution during monotonic cooling of laminated composites
Damage initiation and evolution during monotonic cooling of laminated composites Journal of Composite Materials XX(X):1 38 c The Author(s) 0000 Reprints and permission: sagepub.co.uk/journalspermissions.nav
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationPredicting Failure of Multiangle Composite Laminates
Predicting Failure of Multiangle Composite Laminates Preliminary discussion (not in textbook): Micromechanics failure analyses vs Macromechanics failure analyses Fiber Architecture of Some Common Composite
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationPrediction of Micromechanical Behaviour of Elliptical Frp Composites
Prediction of Micromechanical Behaviour of Elliptical Frp Composites Kiranmayee.Nerusu Dept. of Mechanical Engg. P. V. P. Siddhartha Institute of Technology, Vijayawada 520 007, A.P, India. P. Phani Prasanthi
More informationSchool of Materials Science and Engineering, UNSW Sydney, Australia 2. School of Mechanical and Manufacturing Engineering, UNSW Sydney, Australia
2 st International Conference on Composite Materials Xi an, 2025 th August 207 PREDICTING THE EFFECT OF TEMPERATURE ON MATRIX CRACKING IN THERMOSET COMPOSITES USING A STRAIN INVARIANT APPROACH Akhila
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS. A Thesis. Submitted to the Faculty. Drexel University.
ON HOMOGENIZATION AND DEHOMOGENIZATION OF COMPOSITE MATERIALS A Thesis Submitted to the Faculty of Drexel University by Chang (Karen) Yan in partial fulfillment of the requirements for the degree of Doctor
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationModelling of multiaxial ultimate elastic wall stress (UEWS) test for glass fibre reinforced epoxy (GRE) composite pipes
pplied Mechanics and Materials Vol. 367 (013) pp 113117 Online available since 013/ug/16 at www.scientific.net (013) Trans Tech Publications, Switzerland doi:10.408/www.scientific.net/mm.367.113 Modelling
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationA Constitutive Model for DYNEEMA UD composites
A Constitutive Model for DYNEEMA UD composites L Iannucci 1, D J Pope 2, M Dalzell 2 1 Imperial College, Department of Aeronautics London, SW7 2AZ l.iannucci@imperial.ac.uk 2 Dstl, Porton Down, Salisbury,
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationStatistically Equivalent Representative Volume Elements for Unidirectional Composite Microstructures: Part I Without Damage
Statistically Equivalent Representative Volume Elements for Unidirectional Composite Microstructures: Part I Without Damage SHRIRAM SWAMINATHAN, 1 SOMNATH GHOSH 1, * AND N. J. PAGANO 1,2 1 Department of
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationGetting Started with Composites Modeling and Analysis
Getting Started with Composites Modeling and Analysis IN THIS WEBINAR: PRESENTED BY: Orthotropic materials and how to define them Composite Laminate properties and modeling Composite failure theories and
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationRandom FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Random FiberMatrix Model for Predicting Damage in Multiscale Analysis of Textile Composites under Thermomechanical Loads W. R. McLendon, J. D.
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationTRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES
DEPT. OF MATH., UNIVERSITY OF OSLO RESEARCH REPORT IN MECHANICS, No. 1 ISSN 08019940 December 2012 TRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES by Qiao
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationProgressive Failure Analysis of Laminated Composite Structures
Progressive Failure Analysis of Laminated Composite Structures Arafat Islam Khan Dissertation submitted to the Faculty of the Virginia Polytechnic Institute and State University in partial fulfillment
More informationA FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES
ECCM6 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 24 A FULLY COUPLED MULTISCALE SHELL FORMULATION FOR THE MODELLING OF FIBRE REINFORCED LAMINATES J. Främby, J. Brouzoulis,
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationDynamic analysis of Composite Micro Air Vehicles
Dynamic analysis of Composite Micro Air Vehicles Shishir Kr. Sahu Professor and Head, Civil Engineering, National Institute of Technology, Rourkela, India Email: sksahu@nitrkl.ac.in ABSTRACT The present
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationFatigue Analysis of Wind Turbine Composites using MultiContinuum Theory and the Kinetic Theory of Fracture
Fatigue Analysis of Wind Turbine Composites using MultiContinuum Theory and the Kinetic Theory of Fracture P. Greaves a, P. McKeever a, R. G. Dominy b, T. Koziara b a Narec, Offshore House, Albert Street,
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationEffect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test
Effect of Specimen Dimensions on Flexural Modulus in a 3Point Bending Test M. Praveen Kumar 1 and V. Balakrishna Murthy 2* 1 Mechanical Engineering Department, P.V.P. Siddhartha Institute of Technology,
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More information